(2) JOURNAL OF APPLIED PHYSICS 105, 123907 共2009兲. Surface anisotropy, hysteretic, and magnetic properties of magnetite nanoparticles: A simulation study J. Mazo-Zuluaga,1,a兲 J. Restrepo,1 F. Muñoz,2 and J. Mejía-López2 1. Grupo de Estado Sólido, Grupo de Instrumentación Científica y Microelectrónica, Instituto de Física, Universidad de Antioquia, A.A. 1226, Medellín, Colombia 2 Facultad de Física, Pontificia Universidad Católica, Av. Vicuña Mackenna 4860, Santiago, Chile. 共Received 5 March 2009; accepted 10 May 2009; published online 17 June 2009兲 In this study we address the role of surface anisotropy on the hysteretic properties of magnetite Fe3O4 nanoparticles and the circumstances yielding both horizontal and vertical shifts in the hysteresis loops. Our analysis involves temperature dependence and particle size effects. Different particle sizes ranging from 2 up to 7 nm were considered. Our theoretical framework is based on a three-dimensional classical Heisenberg model with nearest magnetic neighbor interactions involving tetrahedral 共A兲 and octahedral 共B兲 irons. Cubic magnetocrystalline anisotropy for core spins, single-ion site anisotropy for surface spins, and interaction with a uniform external magnetic field were considered. Our results revealed the onset of low temperature exchange bias field, which can be positive or negative at high enough values of the surface anisotropy constant 共KS兲. Susceptibility data, computed separately for the core and the surface, suggest differences in the hard-soft magnetic character at the core-surface interface. Such differences are KS-driven and depend on the system size. Such a hard-soft interplay, via the surface anisotropy, is the proposed mechanism for explaining the observed exchange bias phenomenology. Our results indicate also that the strongly pinned spins at high enough surface anisotropy values are responsible for both the horizontal and vertical shifts in the hysteresis loops. The dependences of the switching and exchange bias fields with the surface anisotropy and temperature are finally discussed. © 2009 American Institute of Physics. 关DOI: 10.1063/1.3148865兴 I. INTRODUCTION. Since the exchange bias was discovered in 1956 by Meiklejohn and Bean,1 most of the reported work on literature has been devoted to the study of layered antiferromagnetic 共AFM兲-ferromagnetic 共FM兲 systems, including mainly, thin films and small particles.2,3 Exchange bias has also been observed in interfaces involving the presence of a ferrimagnet 共ferri兲like AFM-ferri 共Ref. 4兲 and FM-ferri 共Ref. 5兲 systems. However, despite the fact that fine particles were the first type of system where exchange bias was observed, most of the related work on particles deals with those consisting of a FM core surrounded by its respective AFM or ferrimagnetic native oxide,6–10 and some very few studies on pure systems exhibiting exchange bias, e.g., pure ferri or AFM nanoparticles, have been carried out.11,12 In the case for instance of AFM NiO nanoparticles with average size ranging from 5 to 80 nm, large coercivities and shifted hysteresis loops were reported for all samples after field cooling.11 Numerical modeling was also performed in order to endorse the occurrence of multisublattice spin configurations instead of a two-sublattice model. The model was based on considerations of low coordination at surface sites and weak coupling between sublattices, allowing a variety of reversal paths for the spins upon cycling the applied field as a mechanism for exchange bias. Experimental evidence and numerical calculations for organic-coated NiFe2O4 nanoparticles have also a兲. Electronic addresses: firstname.lastname@example.org and email@example.com.. 0021-8979/2009/105共12兲/123907/10/$25.00. demonstrated the occurrence of shifted hysteresis loops after field cooling, consistent with a model of ferrimagnetically aligned core spins and a spin-glasslike surface layer.12,13 Here, nanoparticles were obtained by grinding high purity NiFe2O4 powders in kerosene and oleic acid. Such organic surfactant was found to be strongly bonded to the surface of the nanoparticles. In this case, exchange bias behavior was associated to the existence of many surface canted spin states, one of which is selected by field cooling, separated by energy barriers 共smaller than a certain freezing temperature兲 which can be overcome by thermal activation. An initial study on this kind of nanoparticles revealed an extremely strong spin pinning effect, presumably associated to surface cations bonded to the organic molecules.14 The long-chain surfactant molecules coating the NiFe2O4 particles are known to adsorb via the action of their polar terminal carboxyl group 共⫺COOH兲, which can result in an increase in surface anisotropy. Concerning pure ferrimagnetic magnetite nanoparticles, exchange bias and surface spin-glasslike behaviors have been reported to occur in Fe3O4 nanoparticles compacted under high pressure.15 In the field cooling process a preferred configuration is imposed upon the spin-glasslike surface spins. When the cooling field is removed, the ferrimagnetic core 共with a higher ordering temperature兲 experiences the field generated by the frozen surface spins in the direction of the previously applied field, resulting in a shift in the hysteresis loop, i.e., the hysteresis loop offset arises from the exchange coupling between the spin-glasslike surface and core spins.15 Another related ferrimagnetic oxide system,. 105, 123907-1. © 2009 American Institute of Physics.
(3) 123907-2. Mazo-Zuluaga et al.. namely, ␥-Fe2O3, has also been widely studied from the point of view of hysteretic behavior and exchange bias properties.16–20 Summarizing, those studies suggesting the occurrence of a “surface spin-glasslike state” are consistent with a surface spin disordered layer freezing below certain low temperature and behaving in an entirely different manner from the core. Such a spin-glasslike surface can be thought, in analogy with layered systems, as playing the role of an “AFM” layer surrounding a ferrimagnetic core. However, even though this intuitive picture can seem simple, a full understanding of the exchange bias properties of pure nanoparticles seems to be far beyond standard exchange bias models. Even though studies of bulk ferris with exchange bias behavior have not been systematically carried out, some examples can be found in the literature such as amorphous rare-earth based alloys21,22 and some oxide type ferris.23,24 Magnetite nanoparticles possess some of the characteristics needed for the occurrence of shifted hysteresis loops. On the one hand, the presence of competing interactions can lead to magnetic frustration on the surface due to undercoordination. In magnetite, different superexchange integrals, namely, JAA ⬍ 0, JAB ⬍ 0 and JBB ⬎ 0, are present. The intersublattice JAB superexchange interaction, which is AFM, is dominant and it contributes to the appearance of ferrimagnetic order.25–27 Since such superexchange interactions are mediated by an intervening oxygen ion, exchange bonds are broken if an oxygen is missing from the surface. In consequence, electrons can no longer participate in the superexchange. This fact is important as far as changes in the electric field gradient on the surface can arise. In principle, this can lead to anisotropy which in turn can be either perpendicular or parallel to the surface, depending on the sign of the crystal-field interaction. On the other hand, surface modification, such as the chemical one, can also induce changes in the surface anisotropy and exchange bias properties, as it has been observed in organic-coated NiFe2O4 particles.11,13,14 In particular, magnetite nanoparticles with a chemically modified surface have also been successfully synthesized. An important recent effort in that direction to understand the effect of surfactant coating on the magnetic properties of Fe3O4 nanoparticles, by means of electronic spin resonance 共ESR兲, has been made by Koseoglu.28 In that work, nanoparticles were coated with gold, Na-oleate and methoxypolyethylene glycol. Results showed remarkable differences in the resonance fields and line width of the ESR spectra, indicating strong magnetic surface effects depending on the coating medium. In the same direction, other related works demonstrating the influence of the coating medium on the magnetic properties of magnetite nanoparticles have also been recently addressed.29–31 Hence, it is clear that the matrix where particles can be embedded, the surfactant, the coating medium surrounding the surface of the particles, or even the specific way by which the particle surface ends at atomic level, act as important sources of surface anisotropy. Magnetite has recently been of particular interest for being an excellent candidate for spintronics applications due to the high degree of spin polarization in one of the spin subbands at the Fermi level and at room temperature.32–35 Different facts point out to the surface of magnetite at nanoscale. J. Appl. Phys. 105, 123907 共2009兲. behaving in an entirely different manner than bulk magnetite. Surface studies in magnetite thin films showed the influence of surface morphology, roughness, and stoichiometric inhomogeneities on the electronic structure.36 Ab initio calculations by employing density functional theory 共DFT兲 with the generalized gradient approximation 共GGA兲 and local-density approximation+ U approaches to determine the electronic structure for five different 共111兲 surfaces of Fe3O4 revealed that, depending on the particular cation distribution on the surface, either metallic or half-metallic 共as in bulk Fe3O4兲 behavior can be found.33 A half-metal to metal transition at the 共100兲 Fe3O4 surface has been also observed by means of spin-resolved photoemission experiments on epitaxial and high quality thin films as well as by DFT-GGA calculations.37 Such a half-metal to metal transition has also been confirmed by using first-principles calculations in four different Fe3O4 共001兲 surfaces.38 Different theoretical models and numerical approaches, including recent experimental findings,20 have also been performed in order to contribute to the current understanding of exchange bias in nanoparticles.39–45 Despite all the important amount of papers on this direction, to our knowledge, the effect of the surface anisotropy constant, as a driving force for giving rise to exchange bias in pure ferrimagnetic nanoparticles, has not yet been explored. In this work we present a Monte Carlo study, based on a classical Heisenberg model, to address the effect of surface anisotropy on the exchange bias behavior in magnetite nanoparticles. The layout of the paper is as follows. In Sec. II we introduce the model, the Hamiltonian, describing the interactions to be considered, simulation details, and the observables to be computed. Numerical results and discussions are presented in Sec. III. This section shows 共i兲 the hysteretic properties for different particle diameters and for two different surface anisotropy scenarios, 共ii兲 the effect of strong surface anisotropy upon the hysteretic and exchange bias properties at low temperatures for nanoparticles of 2.5 nm in diameter, and finally 共iii兲 the temperature dependence of the coercive force and susceptibility for two different surface anisotropy values and nanoparticles of 2.5 nm in diameter. Conclusions are finally presented in Sec. IV.. II. MODEL AND MONTE CARLO SIMULATION. The model employed in this study reproduces the inverse spinel crystalline structure of magnetite 共Fe3O4兲 with symmetry Fd3̄m. In this cubic structure a total number of 56 ions per unit cell are considered. They are distributed as follows: 32 O2− oxygen ions, 8 Fe3+ iron ions in tetrahedral sites 共A-sites兲, and finally 8 Fe2+ and 8 Fe3+ ions randomly located in octahedral sites 共B-sites兲. Those iron cations belonging to B-sites are responsible for the nonresolved sextet observed by Mössbauer spectroscopy above the Verwey temperature. Such sextet corresponds to the Fe2.5+ mixed valence state resulting from an electron hopping mechanism between Fe2+ and Fe3+ cations.46 The corresponding chemical formula can be written as.
(4) 123907-3. J. Appl. Phys. 105, 123907 共2009兲. Mazo-Zuluaga et al.. 共Fe3+兲A关Fe2+Fe3+兴BO2− 4 .. 共1兲. Magnetic moments of iron cations were represented by classical Heisenberg spins. Their magnitudes have been considered taking into account their respective valence states and therefore their corresponding electronic configurations, namely, 关Ar兴3d5 for Fe3+ and 关Ar兴3d6 for Fe2+. Thus, a value of S = 5 / 2 was used for Fe3+ and S = 2 for Fe2+. Oxygen ions, which mediate in the superexchange interactions, were considered as nonmagnetic. Spins interact via AFM couplings when considering the following bonds: FeA3+ – FeA3+, FeA3+ – FeB3+, and FeA3+ – FeB2+. By contrast, the following couplings were considered FM: FeB3+ – FeB3+, FeB3+ – FeB2+, and FeB2+ – FeB2+. Numerical values of the integrals employed were JAA = −0.11 meV, JBB = +0.63 meV, and JAB = −2.92 meV.25 Hence, the sign and greater magnitude of the intersublattice integral JAB accounts for antiparallel intersublattice alignment. This fact, in addition to the different spin values, explains the ferrimagnetic behavior observed in bulk magnetite below the Curie temperature. The classical Heisenberg Hamiltonian describing our system can be written as follows: 2 2 2 2 2 Sy,i + S2y,iSz,i + Sx,i Sz,i兲 H = − 2 兺 JijSi · S j − KV 兺 共Sx,i 具i,j典. i. − KS 兺 共Skek兲2 − gBH · 兺 Si . k. 共2兲. i. The first sum involves nearest magnetic neighbors interactions. The number of terms in this sum depends on the coordination numbers. Under bulk conditions three different coordination numbers are identified: zAA = 4, zBB = zBA = 6, and zAB = 12. These numbers apply for the core, whereas the surface is defined as formed by iron ions having coordination numbers smaller than those corresponding to bulk conditions. The second term in Eq. 共2兲 is the core cubic magnetocrystalline anisotropy and KV 共=0.002 meV/ spin兲 is the first-order bulk anisotropy constant.47 The third term accounts for the single-ion site surface anisotropy where the unitary vector ek is computed on every kth position taking into account the positions P j of the nearest magnetic neighbors.48 ek =. 兺 j 共Pk − P j兲 . 兩 兺 j 共Pk − P j兲兩. 共3兲. Positions over which these vectors were computed correspond exclusively to Fe-cations on the surface. The last term in Eq. 共2兲 gives the interaction of spins with a uniform external magnetic field. Estimates of the different energies involved, including dipole-dipole interactions over the entire volume, were initially performed. Such estimates yielded the following orders of magnitude: ⬃103 meV/ spin for superexchange interactions, ⬃10−2 meV/ spin for surface anisotropy, ⬃10−4 meV/ spin for cubic anisotropy, and ⬃10−5 meV/ spin for dipole-dipole interactions. Therefore, dipolar interactions were neglected in the present study.49 Regarding the Monte Carlo simulation, we have employed a single-spin movement Metropolis dynamics. Averages were computed over 25 different samples corresponding to five. different magnetic starting configurations and five different realizations of Fe3+ and Fe2+ ions at octahedral sites per each initial magnetic configuration. Hence, error bars were computed. A maximum number of 5 ⫻ 105 Monte Carlo steps per spin 共MCS兲 were used and the first 2 ⫻ 105 steps were discarded for equilibration. The lowest temperature considered was 10 K and no special considerations on crystalline symmetry were made for temperatures below the Verwey temperature TV known to be at around 120 K for bulk magnetite. The reason for this is experimentally endorsed by several studies in which the suppression of the Verwey transition takes place for particle sizes below 20 nm.47,50,51 We want to stress however that investigations on magnetite nanoparticles with monoclinic symmetry are currently under progress. Numerical values for the KS / KV ratio were taken to range between 1 and 104. Such extreme values allow: 共i兲 to determine the stability of the magnetic structures involved and 共ii兲 to model different experimental and likely scenarios where a given matrix or coating medium, such as an organic surfactant, can effectively change the surface anisotropy. Some few simulation studies addressing the effect of strong surface anisotropy can be found in the literature.49,52–61 Nearly spherical nanoparticles of different diameters were considered: D = 2, 2.5, 3.0, 3.5, 4, 4.5, 5, 6, and 7 nm. Free boundary conditions were implemented and the thermodynamic quantities computed were the energy, the magnetization per spin, the magnetic susceptibility, and the specific heat. Contributions to the total magnetization, magnetic susceptibility, and hysteresis loops, arising from A and B sites, as well as from core and surface, were separately computed. III. RESULTS AND DISCUSSION A. Hysteresis loops for low surface anisotropy. In order to study the effect of particle size on the hysteretic properties temperature was set to 10 K and KS / KV = 10. Hysteresis loops for different particle diameters are shown in Fig. 1. Cycles are characterized by a high degree of squareness, associated with the reversal of the magnetization as a whole, and a marked tendency of the saturation magnetization and the remanence to decrease as the particle size decreases. Under bulk conditions the saturation magnetization per spin goes to 2/3 accordingly with stoichiometry and the different Fe spin values involved. Values close to this limit were obtained for nanoparticles of 6 and 7 nm in diameter, whereas finite size effects become evident for smaller nanoparticles having smaller values of the saturation magnetization per spin. Here, magnetization reduction is due to uncompensated spins on the surface and not to a surface spin canting phenomenology. Moreover, in the remanence and the saturation states magnetic structure is characterized by an almost perfect ferrimagnetic alignment of the spins in the entire volume of the nanoparticle for the considered surface anisotropy value 共Fig. 2兲. By plotting separately the core and surface contributions to the total magnetization, as shown in Fig. 3, for a given particle size, both the loops of the core and the surface are almost square. This result holds independently of the particle size for KS / KV = 10. This result implies a reversal of the mag-.
(5) 123907-4. Mazo-Zuluaga et al.. FIG. 1. 共Color online兲 Hysteresis loops at 10 K and KS / KV = 10 for different particle sizes. Both coercive force and remanence tend to diminish as the particle size decreases.. netization as a whole with a well-defined ferrimagnetic moment, i.e., nanoparticles behave like macrospins, as in the Stoner–Wohlfarth model.49 Additionally, it is the reversal of the surface spins which triggers the reversal of the core. This is indicated by the fact that the switching field of the surface is slightly smaller to the one of the core 共open circles in Fig. 3兲. Concerning exchange bias properties at these low KS values, no shifted loops can be confirmed within the degree of precision provided by the error bars. As the surface anisotropy increases hysteresis loops become substantially different. Figure 4 shows the hysteresis loops for different particle diameters at T = 10 K and KS / KV = 3000. In this case, hysteresis loops remain symmetric but different from those cycles at smaller surface anisotropy values, hysteresis loops now appear less square and more elongated. Remanence reduction becomes now more remarkable as the particle size decreases. This fact is mainly. FIG. 2. 共Color online兲 Surface magnetic structure for a nanoparticle of 3 nm at 10 K and KS / KV = 10. Ferrimagnetic alignment is preserved both on the surface and in the core. Arrows represent Fe spins: gray 共red兲 color for Fe3+ A ions 共pointing to the left兲, dark gray 共blue兲 for Fe3+ B ions, and light gray 共green兲 for Fe2+ B 共both of them pointing to the right兲.. J. Appl. Phys. 105, 123907 共2009兲. FIG. 3. 共Color online兲 Total 共T兲, surface 共S兲, and core 共C兲 contributions to the hysteresis loop for D = 3.5 nm at T = 10 K and KS / KV = 10. Similar results were obtained for all the particle sizes. Coercive force of the surface is slightly smaller than that of the core 共open circles兲.. due to a small tendency of the surface spins to be pinned along radial directions for which magnetic structures are of the throttled type.55,58 Figure 5 shows the variation with the particle diameter of the coercive force for the two surface anisotropy values above considered. As can be observed, coercivity displays an increasing monotonic size dependence whose slope changes depending on the surface anisotropy. For KS / KV = 3000 the switching field follows the same increasing behavior as the particle size increases, but now the obtained values are greater by keeping the same conditions than those obtained for KS / KV = 10. The reason for that is the increase, via KS, in the height of the energy barrier to be overcome. Even though the reversal of magnetization can be considered coherent, deviations from the number of core spins relative to the total 共Nc / N兲 are observed. This means that only those particles. FIG. 4. 共Color online兲 Hysteresis loops at 10 K and KS / KV = 3000 for different particle sizes. Coercive force diminishes as the particle size decreases..
(6) 123907-5. Mazo-Zuluaga et al.. FIG. 5. 共Color online兲 Low temperature coercive force as a function of the particle diameter for two different KS / KV ratios. Dashed lines are guides to the eyes.. with small surface anisotropy and bigger size behave accordingly with the Stoner–Wohlfarth model.49 As the particle size is reduced the density of magnetic bonds decreases as long as the proportion of undercoordinated ions on the surface becomes greater. Thus, smaller fields enable more easily the reversal of spins and lead to lower switching fields for smaller sizes. In order to evaluate separately the core and surface behaviors regarding the hysteretic properties for KS / KV = 3000, Fig. 6 shows the core and surface contributions to the hysteresis loops for a 2.5 nm nanoparticle and KS / KV = 3000. Results indicate a progressive reversal of the surface magnetization which is a typical feature associated with disordered or frustrated systems. Analogously to what was observed for. J. Appl. Phys. 105, 123907 共2009兲. FIG. 7. Dependence of the magnetization with the KS / KV ratio at T = 10 K for nanoparticles of D = 2.5 nm.. KS / KV = 10, the reversal of the surface spins triggers the reversal of the core, and the core magnetization tends to be reversed as a whole besides being saturable. It must be stressed that most of the zero-field magnetic structures for the range of values of KS / KV considered up to here are characterized for having a well-defined ferrimagnetic alignment along the 共111兲 direction for KS / KV = 10 共Fig. 2兲, whereas for KS / KV = 3000 the magnetic structure is of the throttled type55,58 where it is more noticeable the tendency of surface spins to be perpendicular to the surface. For greater surface anisotropy values beyond certain threshold, which depends on the system size, magnetic structures become of the hedgehog type with magnetization close to zero. Figure 7 shows the dependence of the zero-field magnetization with the surface anisotropy over a wide range of values for nanoparticles of 2.5 nm in diameter. A KS-driven magnetic transition is observed, where for values above KS / KV ⬇ 3500 the magnetic structure is of the hedgehog type, as that shown in Fig. 8. B. Hysteresis loops for high surface anisotropy. FIG. 6. 共Color online兲 Total 共T兲, surface 共S兲, and core 共C兲 contributions to the hysteresis loop for D = 2.5 nm at T = 10 K and KS / KV = 3000.. Concerning exchange bias properties, shifted loops were evidenced for nanoparticles having some specific ranges of high enough surface anisotropy values above KS / KV = 3000, as can be observed in Fig. 9, for a nanoparticle of 2.5 nm. Exchange bias can be understood in terms of the different paths followed by the core and surface spins during the reversal process of the magnetization. High values of the surface anisotropy constant make the surface spins to be pinned and consequently the surface becomes magnetically hard during the reversal process. This is the reason for the progressive reversal of the surface magnetization and the high degree of irreversibility upon cycling the applied field. Contrary to this, the core of the nanoparticle, where the anisotropy remains fixed and much smaller than that of the surface, behaves in a softer manner. Such a hard-soft interplay.
(7) 123907-6. Mazo-Zuluaga et al.. FIG. 8. 共Color online兲 Magnetic structure for a nanoparticle of D = 3 nm at T = 10 K and KS / KV = 7000. Arrows represent Fe spins: gray 共red兲 color for 3+ Fe3+ A ions 共inwards兲, dark gray 共blue兲 for FeB ions, and light gray 共green兲 for 2+ FeB 共both of them outwards兲.. between surface and core gives rise to the occurrence of an interface across which surface and core spins interact via superexchange couplings. On the other hand, uncompensated spins on the surface, where different spin values are involved, are not necessarily symmetrically distributed due to the finiteness and discreteness of the system. This fact is more evident for smaller nanoparticles. Such spins, strongly pinned, tend to exert a microscopic torque on the core spins. Once the field is applied some of those torques become favored, depending on the direction along which the field is applied. As a result, and due to the nonsymmetric distribution of such torques, a hysteresis loop shift, which can be positive or negative, will be observed along the field axis. Similar mechanisms for explaining exchange bias properties have been also suggested to occur in oxide-coated manganese nanoparticles.57 The evidence for the occurrence of such torques has been already demonstrated in previous studies at. FIG. 9. 共Color online兲 Hysteresis loops for nanoparticles of D = 2.5 nm at T = 10 K and different KS / KV values.. J. Appl. Phys. 105, 123907 共2009兲. FIG. 10. 共Color online兲 Dependence of both the exchange bias and coercive force with the surface anisotropy for nanoparticles of 2.5 nm in diameter and T = 10 K.. zero field, where the tendency of the surface spins to be radially oriented is propagated through the core via superexchange couplings giving rise to hedgehog-type magnetic states, as that shown in Fig. 8.55,57,58 Summarizing, the tendency of the surface spins to be more or less compensated, depending on the particle size, in addition to the different ratio of octahedral to tetrahedral spins,62 explains why the values of surface anisotropy for which exchange bias appears, and it can be positive or negative, are different for different system sizes. Figure 10 shows both the dependence of exchange bias and coercive force as a function of KS / KV. As can be observed, for intermediate values of the ratio KS / KV around 4200, a negative exchange bias is observed, whereas for higher values of this ratio around 9000 exchange bias becomes positive. Such a particular scenario can be understood by analyzing the different contributions to the total magnetization in the hysteresis loops as can be observed in Figs. 11–13 for three different KS / KV values. At around KS / KV ⬇ 4200, once the magnetization of octahedral sites, which is the major contribution to the total magnetization, is reversed when passing from point c to d in Fig. 11, some of the FeB spins remain pinned and relatively unaffected with a projection along the field axis opposite to the field direction. Such spins store energy like a torsion spring and they exert an additional torque on the reversible spins. This fact implies that the following magnetization reversal, from point g to h, takes place at lower fields resulting in a negative exchange bias. This can be concluded because the magnitude of the magnetization in the positive field direction is larger than that in the opposite direction, which indicates that some of the spins are pinned in the positive field direction and cannot be reversed by the field. The difference between these two magnetizations is proportional to the number of pinned spins. Moreover, the zero-field magnetization 共remanence兲 at point b is greater in magnitude than that at point f where the unreversed spins make the absolute value of the magnetization be smaller re-.
(8) 123907-7. Mazo-Zuluaga et al.. J. Appl. Phys. 105, 123907 共2009兲. FIG. 11. 共Color online兲 Total 共T兲, surface 共S兲, core 共C兲, tetrahedral 共A兲, and octahedral 共B兲 contributions to the hysteresis loops for D = 2.5 nm, T = 10 K, and KS / KV = 4.2⫻ 103.. FIG. 13. 共Color online兲 Total 共T兲, surface 共S兲, core 共C兲, tetrahedral 共A兲, and octahedral 共B兲 contributions to the hysteresis loops for D = 2.5 nm, T = 10 K, and KS / KV = 9 ⫻ 103.. sulting in turn in an upwards magnetization vertical shift. Concurrently, the contribution to the hysteresis loops from FeA spins undergoes a downwards vertical shift as a consequence of the intersublattice AFM coupling, which is larger than the intrasublattice coupling. As the surface anisotropy increases, the tendency of the surface spins to be perpendicular to the surface begins to propagate to the core via superexchange couplings. This fact makes the overall system magnetically harder and consequently the coercive force increases. At this stage the gradual reversal of the magnetization is complete, i.e., there are not unreversed spins, giving rise to a symmetry at both negative and positive fields, and therefore no exchange bias is observed 共Fig. 12兲. As we go further in the value of surface anisotropy at around KS / KV. ⬇ 9000, a downwards vertical shift in the FeB spins cycle appears, giving rise to a positive exchange bias 共Fig. 13兲. This fact can be understood as due to the interplay between the Zeemann energy and the surface anisotropy for which the amount of unreversed spins increases again. Differently from the earlier stage at lower KS / KV values, more unreversed spins are aligned or closely aligned opposite to the positive field direction, and those spins with anisotropy axis perpendicular or closely perpendicular to the field axis are forced to follow the field direction. Once the field is reversed, those spins pinned along the negative field direction exert an additional torque on the reversible FeB spins resulting in a positive exchange bias. Cycles reveal also that nucleation begins before switching the field in correspondence with a high degree of irreversibility. This behavior differs from that observed at low KS / KV values below 3000, where the symmetry in the magnetization values both at positive and negative fields indicates the absence of pinned spins 共Fig. 1兲. It must be stressed at this point that the distribution of pinned spins is not symmetric. Finally, for huge values of KS / KV above 9000, the hedgehog-type magnetic structure becomes practically rigid giving rise to the absence of both coercivity and exchange bias 共Fig. 10兲. Hysteresis loops are characterized by steps or jumps, which become more pronounced as the surface anisotropy increases. Such jumps are attributed to the high degree of spin pinning, for which reversal does not occur in a continuous fashion, and to a discrete shift in the center of symmetry of the magnetic moment distribution in the direction opposite to the field.55 As is well established, in order to generate exchange bias it is necessary to have the presence of at least two exchange-coupled phases: a reversible phase whose magnetic moments can be reversed and a fixed phase whose moments cannot be reversed. In our case those pinned spins, which belong to the surface or even to the core, play the role of the fixed phase. On the other hand, the reversible phase includes both the contributions of the. FIG. 12. 共Color online兲 Total 共T兲, surface 共S兲, core 共C兲, tetrahedral 共A兲, and octahedral 共B兲 contributions to the hysteresis loops for D = 2.5 nm, T = 10 K, and KS / KV = 6.5⫻ 103..
(9) 123907-8. Mazo-Zuluaga et al.. core and the reversible part of the surface. The relative proportion of each phase will depend on the magnitude of the surface anisotropy. Summarizing, exchange bias results from the coupling between the pinned spins, strongly influenced by the surface anisotropy, and the reversible spins. Experimentally, vertical shifts have been recently reported to occur in similar systems to the one considered here such as CoFe2O4 nanoparticles.63 Here, vertical shifts, accompanying the exchange bias, were associated with the presence of strongly pinned uncompensated spins at the core-shell interface. Analogously, frozen spins in ␥-Fe2O3 coated Fe nanoparticles are responsible for both horizontal and vertical shifts in the hysteresis loops.64 In this last case, it is a spinglasslike phase with high-field irreversibility in the ␥-Fe2O3 shell that plays the role of the fixed phase. Large shifts in both horizontal and vertical directions have also been found in milled Fe/ MnO2 systems65 having some similarities to the one studied here where shifts were attributed to a large surface contribution of a noncollinear magnetic structure. In short, as the surface anisotropy increases the magnetization reversal process becomes progressively gradual. For KS / KV ratios above certain threshold value of approximately 5 ⫻ 103, several features are remarkable: 共i兲 cycles are widely elongated and open up to approximately the maximum applied field, 共ii兲 magnetization reversal occurs step by step, suggesting a distribution of switching fields or rotational barriers, 共iii兲 it is the reversal of the surface spins which triggers the reversal of the core, and 共iv兲 exchange bias properties appear. Once the field is applied on a hedgehog-type nanoparticle, very high fields are required to force transitions between surface spins and to overcome the high degree of pinning of the magnetic moments. This fact explains the highfield irreversibility. In literature some results have been reported for NiFe2O4 nanoparticles showing the persistence of hysteresis up to 16 T, 400 times larger than the bulk magnetocrystalline anisotropy field.13 Exchange bias and the presence of jumps during magnetization reversal are also attributed to the high degree of surface spin pinning. In our case, surface spin pinning is relevant at high enough surface anisotropy values above the threshold when such behavior tends to propagate through the core via superexchange couplings.. J. Appl. Phys. 105, 123907 共2009兲. FIG. 14. 共Color online兲 Temperature dependence of the coercivity for two different KS / KV ratios and D = 2.5 nm.. different manner. This phenomenology resembles a phase separation process and suggests that the phase transition takes place in a very gradual fashion. In the case of very high anisotropy values 共see Fig. 16兲, results reveal a marked tendency to diverge in a very narrow range of temperature. This feature is attributed to the sharp transition to the hedgehog structure characterized by a magnetization close to zero in the low temperature regime. Finally, we want to comment that coercive force values obtained through simulation cannot be directly compared to those experimentally reported. As is well established experimentally as well as numerically, the coercivity depends on the speed at which the applied field is varied. In Monte Carlo simulations that speed is determined by the number of Monte Carlo steps employed in computing the ensemble averages and the field step size during the cycle. That means that, in principle, it is possible to tune the number of MCS and field step size in order to obtained values similar to those experi-. C. Thermal Effects. Figure 14 shows the temperature dependence of the coercivity for two different KS / KV ratios and D = 2.5 nm. Coercivity decreases with increasing temperature and vanishes at around 450 K. Contrary to this, exchange bias remains almost zero 共within the error bars兲. Another important feature that allows us to understand the already mentioned hard-soft interplay between surface and core is illustrated finally in Figs. 15 and 16. These figures show the surface and core contributions to the total magnetic susceptibility as a function of temperature for a nanoparticle of D = 2.5 nm, two different KS / KV ratios, and zero field. The fact that the temperature at which the surface susceptibility reaches the maximum is lower than that found at the core indicates that both surface and core behave in a. FIG. 15. 共Color online兲 Temperature dependence of the total susceptibility, core and surface contributions for nanoparticles of 2.5 nm in diameter and KS / KV = 10..
(10) 123907-9. J. Appl. Phys. 105, 123907 共2009兲. Mazo-Zuluaga et al.. ACKNOWLEDGMENTS. This study was supported by the Sostenibilidad projects of the GES and GICM groups and the CODI Project No. IN565CE at the Universidad de Antioquia, FONDECYT Grant Nos. 1050066 and 7080111, and the “Millenium Science Nucleus, Basic and Applied Magnetism Grant No. P06022F” project. One of the authors 共J.M.Z兲 wishes to thank Universidad de Antioquia and COLCIENCIAS for their support. W. H. Meiklejohn and C. P. Bean, Phys. Rev. 102, 1413 共1956兲; 105, 904 共1957兲. 2 J. Nogués and I. K. Schuller, J. Magn. Magn. Mater. 192, 203 共1999兲. 3 J. Nogués, J. Sort, V. Langlais, V. Skumryev, S. Suriñach, J. S. Muñoz, and M. D. Baró, Phys. Rep. 422, 65 共2005兲. 4 P. J. Van der Zaag, R. M. Wolf, A. R. Ball, C. Bordel, L. F. Feiner, and R. Jungblut, J. Magn. Magn. Mater. 148, 346 共1995兲. 5 W. C. Cain and M. H. Kryder, J. Appl. Phys. 67, 5722 共1990兲. 6 M. Spasova, U. Wiedwald, M. Farle, T. Radetic, U. Dahmen, M. Hilgendorff, and M. Giersig, J. Magn. Magn. Mater. 272–276, 1508 共2004兲. 7 D. S. Geoghegan, P. G. McCormick, and R. Street, Mater. Sci. Forum 179–181, 629 共1995兲. 8 W. H. Meiklejohn, J. Appl. Phys. 29, 454 共1958兲. 9 V. Papaefthymiou, A. Kostikas, A. Simopulos, D. Niarchos, S. Gangopadhyay, G. C. Hadjipanayis, C. M. Sorensen, and K. J. Klabunde, J. Appl. Phys. 67, 4487 共1990兲. 10 C. M. Hsu, H. M. Lin, and K. R. Tsai, J. Appl. Phys. 76, 4793 共1994兲. 11 R. H. Kodama, A. E. Berkowitz, E. J. McNiff, Jr., and S. Foner, J. Appl. Phys. 81, 5552 共1997兲. 12 R. H. Kodama, S. A. Makhlouf, and A. E. Berkowitz, Phys. Rev. Lett. 79, 1393 共1997兲. 13 R. H. Kodama, A. E. Berkowitz, E. J. McNiff, and S. Foner, Phys. Rev. Lett. 77, 394 共1996兲. 14 A. E. Berkowitz, J. A. Lahut, I. S. Jacobs, L. M. Levinson, and D. W. Forester, Phys. Rev. Lett. 34, 594 共1975兲. 15 H. Wang, T. Zhu, K. Zhao, W. N. Wang, C. S. Wang, Y. J. Wang, and W. S. Zhan, Phys. Rev. B 70, 092409 共2004兲. 16 B. Martínez, X. Obradors, L. Balcells, A. Rouanet, and C. Monty, Phys. Rev. Lett. 80, 181 共1998兲. 17 E. Tronc, D. Fiorani, M. Nogués, A. M. Testa, F. Lucari, F. D’Orazio, J. M. Grenèche, W. Wernsdorfer, N. Galvez, C. Chanéac, D. Mailly, M. Verdager, and J. P. Jolivet, J. Magn. Magn. Mater. 262, 6 共2003兲. 18 C. Frandsen, C. W. Ostenfeld, M. Xu, C. S. Jacobsen, L. Keller, K. Lefmann, and S. Morup, Phys. Rev. B 70, 134416 共2004兲. 19 Ó. Iglesias and A. Labarta, Physica B 343, 286 共2004兲. 20 A. Cabot, A. Paul Alivisatos, V. F. Puntes, L. Balcells, Ó. Iglesias, and A. Labarta, Phys. Rev. B 79, 094419 共2009兲. 21 G. L. Bona, F. Meier, H. C. Siegmann, and R. J. Gambino, Appl. Phys. Lett. 52, 166 共1988兲. 22 E. V. Shipil’, K. Y. Guslienko, and B. Szymanski, IEEE Trans. Magn. 30, 797 共1994兲. 23 N. Sakamoto, J. Phys. Soc. Jpn. 17, 99 共1962兲. 24 Y. Suzuki, R. B. Van Dover, E. M. Gyorgy, J. M. Phillips, V. Korenivski, D. J. Werder, C. H. Chen, R. J. Felder, R. J. Cava, J. J. Krajewski, and W. F. Peck, Jr., J. Appl. Phys. 79, 5923 共1996兲. 25 M. Uhl and B. Siberchicot, J. Phys.: Condens. Matter 7, 4227 共1995兲. 26 P. G. Bercoff and H. R. Bertorello, J. Magn. Magn. Mater. 169, 314 共1997兲. 27 C. M. Srivastava, G. Srinivasan, and N. G. Nanadikar, Phys. Rev. B 19, 499 共1979兲. 28 Y. Koseoglu, J. Magn. Magn. Mater. 300, e327 共2006兲. 29 M. Timko, M. Koneracká, N. Tomasovicová, P. Kopcanský, and V. Závisová, J. Magn. Magn. Mater. 300, e191 共2006兲. 30 P. Guardia, B. Batlle-Brugal, A. G. Roca, O. Iglesias, M. P. Morales, C. J. Serna, A. Labarta, and X. Batlle, J. Magn. Magn. Mater. 316, e756 共2007兲. 31 A. F. Bakuzis, A. R. Pereira, J. G. Santos, and P. C. Morais, J. Appl. Phys. 99, 08C301 共2006兲. 32 E. Arisi, I. Bergenti, M. Cavallini, M. Murgia, A. Riminucci, G. Ruani, and V. Dediu, J. Magn. Magn. Mater. 316, 410 共2007兲. 33 L. Zhu, K. L. Yao, and Z. L. Liu, Phys. Rev. B 74, 035409 共2006兲. 34 Y. J. Kim, C. Westphal, R. X. Ynzunza, H. C. Galloway, M. B. Salmeron, 1. FIG. 16. 共Color online兲 Temperature dependence of the total susceptibility, core and surface contributions for nanoparticles of 2.5 nm in diameter and KS / KV = 7000.. mentally achievable, but that demands a huge computational effort. Similar values for the field range have been, for instance, reported elsewhere.55 However, we want to stress that the conditions 共MCS and field step兲 under which our hysteresis loops were recorded remained fixed in all the cases, which allows comparison among them. Comparisons with experiment are also difficult as far as hysteresis loops for an isolated magnetite nanoparticle have to date not been reported, and those found in the literature correspond to assemblies of interacting nanoparticles.47 IV. CONCLUSIONS. The effect of surface anisotropy and particle size on the hysteretic and magnetic properties of magnetite nanoparticles has been addressed. Results revealed that the magnitude of the surface anisotropy constant can act as a driving force giving rise to the occurrence of a strong surface spin pinning. Exchange bias behavior, which can be positive, negative, or even a vanishing value depending on the particle size, can be attributed to the tendency of the surface spins to be more or less compensated and to the different ratio of octahedral to tetrahedral spins. The pinning mechanism is also the one responsible for magnetization and remanence reduction. Moreover, nanoparticles with a giant surface anisotropy can exhibit, at zero field, spin structures of the hedgehog type characterized by a magnetization close to zero in the low temperature regime. Finally, the differentiated analysis of the core and surface contributions to the total susceptibility allows us to conclude that both regions behave in a different manner resembling a magnetic phase separation process of the hard-soft type, and giving rise to a gradual transition from the ferrimagnetic to the paramagnetic state. More specifically, susceptibility data suggest a magnetically harder character for the surface relative to the core as the surface anisotropy increases. Such a coupled hard-soft interplay is the proposed mechanism for explaining the onset of exchange bias behavior..
(11) 123907-10. M. A. Van Hove, and C. S. Fadley, Phys. Rev. B 55, R13448 共1997兲. S. K. Park, T. Ishikawa, and Y. Tokura, Phys. Rev. B 58, 3717 共1998兲. 36 K. Jordan, A. Cazacu, G. Manai, S. F. Ceballos, S. Murphy, and I. V. Shvets, Phys. Rev. B 74, 085416 共2006兲. 37 M. Fonin, R. Pentcheva, Yu. S. Dedkov, M. Sperlich, D. V. Vyalikh, M. Scheffler, U. Rüdiger, and G. Güntherodt, Phys. Rev. B 72, 104436 共2005兲. 38 C. Cheng, Phys. Rev. B 71, 052401 共2005兲. 39 Ó. Iglesias, X. Batlle, and A. Labarta, Phys. Rev. B 72, 212401 共2005兲. 40 E. Eftaxias and K. N. Trohidou, Phys. Rev. B 71, 134406 共2005兲. 41 Ó. Iglesias and A. Labarta, Physica B 372, 247 共2006兲. 42 K. N. Trohidou, M. Vasilakaki, L. Del Bianco, D. Fiorani, and A. M. Testa, J. Magn. Magn. Mater. 316, e82 共2007兲. 43 D. Kechrakos, K. N. Trohidou, and M. Vasilakaki, J. Magn. Magn. Mater. 316, e291 共2007兲. 44 Ó. Iglesias, X. Batlle, and A. Labarta, J. Magn. Magn. Mater. 316, 140 共2007兲. 45 M. H. Wu, Q. C. Li, and J.-M. Liu, J. Phys.: Condens. Matter 19, 186202 共2007兲. 46 E. De Grave, R. M. Persoons, R. E. Vandenberghe, and P. M. A. de Bakker, Phys. Rev. B 47, 5881 共1993兲. 47 G. F. Goya, T. S. Berquó, F. C. Fonseca, and M. P. Morales, J. Appl. Phys. 94, 3520 共2003兲. 48 R. H. Kodama and A. E. Berkowitz, Phys. Rev. B 59, 6321 共1999兲. 49 H. Kachkachi and M. Dimian, Phys. Rev. B 66, 174419 共2002兲. 50 J. Wang, Q. Chen, X. Li, L. Shi, Z. Peng, and C. Zeng, Chem. Phys. Lett. 390, 55 共2004兲. 35. J. Appl. Phys. 105, 123907 共2009兲. Mazo-Zuluaga et al. 51. N. A. Fellenz, S. G. Marchetti, J. F. Bengoa, R. C. Mercader, and S. J. Stewart, J. Magn. Magn. Mater. 300, 60 共2006兲. 52 D. A. Garanin and H. Kachkachi, Phys. Rev. Lett. 90, 065504 共2003兲. 53 H. Kachkachi and H. Mahboub, J. Magn. Magn. Mater. 278, 334 共2004兲. 54 Ó. Iglesias and A. Labarta, J. Magn. Magn. Mater. 272–276, 685 共2004兲. 55 L. Berger, Y. Labaye, M. Tamine, and J. M. D. Coey, Phys. Rev. B 77, 104431 共2008兲. 56 P. Z. Si, D. Li, J. W. Lee, C. J. Choi, Z. D. Zhang, D. Y. Geng, and E. Brück, Appl. Phys. Lett. 87, 133122 共2005兲. 57 Y. Labaye, O. Crisan, L. Berger, J. M. Greneche, and J. M. D. Coey, J. Appl. Phys. 91, 8715 共2002兲. 58 J. Mazo-Zuluaga, J. Restrepo, and J. Mejía-López, J. Appl. Phys. 103, 113906 共2008兲. 59 J. Mazo-Zuluaga, J. Restrepo, and J. Mejía-López, Physica B 398, 187 共2007兲. 60 J. Restrepo, Y. Labaye, and J. M. Greneche, Physica B 384, 221 共2006兲. 61 J. Restrepo, Y. Labaye, L. Berger, and J. M. Greneche, J. Magn. Magn. Mater. 272–276, 681 共2004兲. 62 J. Mazo-Zuluaga, J. Restrepo, and J. Mejía-López, J. Phys.: Condens. Matter 20, 195213 共2008兲. 63 A. Mumtaz, K. Maaz, B. Janjua, S. K. Hasanain, and M. F. Bertino, J. Magn. Magn. Mater. 313, 266 共2007兲. 64 R. K. Zheng, G. H. Wen, K. K. Fung, and X. X. Zhang, Phys. Rev. B 69, 214431 共2004兲; J. Appl. Phys. 95, 5244 共2004兲. 65 E. C. Passamani, C. Larica, C. Marques, J. R. Proveti, A. Y. Takeuchi, and F. H. Sánchez, J. Magn. Magn. Mater. 299, 11 共2006兲..